100 Views

Download Presentation
##### Bias Fields and Pattern Complexity

**An Image/Link below is provided (as is) to download presentation**

Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author. While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

- - - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - - -

**Bias Fields and Pattern Complexity**M.E. Glicksman Allen S. Henry Professor of Engineering Mechanical & Aerospace Engineering Dept. Florida Institute of Technology, Melbourne, FL Presentation at the UCLA Institute for Pure & Applied Mathematics Los Angeles, CA November 13, 2012**Outline**Pattern formation & microstructures Early experiments & conventional ideas Surprises from microgravity experiments Conservation of energy Capillarity, more than a boundary condition! Bias fields: Why did we miss it? Dynamic simulations**Motivation & Associated Questions**Complex pattern evolution occurs throughout nature, society, and technology. Self-organized patterns remain important in areas as diverse as cosmology, meteorology, biology, and engineering. Branching (ramification and splitting) allows simple starting forms to achieve increasing complexity. Is there a causal principle responsible for branching and surface diffusion? Where does the information driving complexity reside ? Is pattern branching fundamentally stochastic or deterministic ?**Self-Organized Branching Patterns**Dendritic Superalloy Turbine blades Jet engine efficiency Microstructure control Mechanical properties Improved creep resistance Polycrystal Directional Monocrystal Bio-iridescence Electro-magnetic diffraction Photonic (chiten) dendrites Sensitive chemical probes Pigmentless paints & coatings Dendritic Photonic Array MorphoRetenor**Phase-Field Simulated Cu-Au DendriteCourtesy of J. Warren &**W. Boettinger, NIST • Sophisticated modeling—but: • Noise is considered essential—?? • Modelers unaware of a basic mechanism • Pattern optimization & control limited • Missing link is the interface ‘bias field’**Pattern Evolution**Dendrites: Casting, welding, primary metals production, crystal growth ‘Seaweed’: Fluid-fluid penetration, Hele-Shaw patterns, petroleum recovery, biogenesis What’s causal?**Pattern Size & Supercooling**ΔT=6.82 K V= 3.65 cm/s ΔT=4.61 K V= 1.25 cm/s ΔT=4.00 K V= 0.86 cm/s 7-9s SCN • Solid-liquid interface is a source of heat/solute 40 micron • Energy/solute released must be transported away • Boundary conditions: capillarity, kinetics, and T • Branches appear periodically, develop irregularities • Noise and stability responsible for pattern formation. ΔT=3.00 K V= 0.38 cm/s ΔT=2.00 K V= 0.14 cm/s ΔT=1.25 K V= 0.032 cm/s**NASA Microgravity Experiments**Melting Provided the big clue on pattern formation! Solidification • IDGE Experiments • Field Theory • Numerics • Bias Field Analysis • Dynamic simulation • Conclusions**Precision thermostat: (0.002 K)**35mm camera Xenon flash Red LED CCD camera Sample chamber USMP-4/IDGE Space Flight Instrument**Dendritic Growth in Space**(PVA, ΔT=1.2K)**Analysis of Melting in Microgravity**• Field Theory—a few words • Coordinate system • Laplace field • Origin of self-similarity • Melting kinetics**=1**0.9 0.75 0.5 0.25 C/A=20 =2 1.6 1.3 1.1 1 1.03 0 -0.25 -0.5 -0.75 -0.9 =-1 Confocal ProlateSpheroidal Coordinates • A. Lupulescu, M.E. Glicksman, and M.B. Koss, • J. Thermophysics and Heat Transfer,17, (2002) Exterior potential =0 Interior potential**Self-Similar Melting (9:1Ellipsoid)**Self-similarity C/A time Vector gradient fields: Isothermal interface**Melting ‘Trajectory’(St+=0.036, C/A=15, C0 =0.76cm,**Ξ=1.0026)**C/A versus Time: Big surprise!**Not self-similar ? Self-similar**Self-similarity**TTTTint ≠ const. TTTTint =const. ≥ • Gibbs-Thomson bcimposed • Tint now depends on curvature, κ • We found: • • Interior heat flow • • Capillary-mediated fluxes • • Non self-similar melting! • Numerical (Finite Difference) no capillarity, Dr. S. Salon, RPI**Gibbs-Thomson-Herring Potential**anisotropic isotropic Convex Gamma Plots Avoids equilibrium facets**Global vs. Local Thermodynamic Equilibrium**Global equilibrium: Strong condition that minimizes Gibbs free energy in closed systems equilibrium Initial state equilibrium Allow dynamics: Local equilibrium: Weak condition that reduces free energy in open systems bias field Initial state bias field Allow dynamics:**Energy Conservation2-Phase Domain Contraction**N n S(t) c D(t) Domain Contraction n S(t)**Interface Energy Conservation (Leibniz-Reynolds &**Kelvin-Stokes thms) N n S(t) c D(t) (Domain contraction) (Meso-scale) (Local equilibrium) (Fourier’s law )**Interface Energy Conservation**Definitions Ref. Mod. Bias Field Modulation Interface Poisson Eqn.**Branch Initiation: A non-self similar event, suggesting a**2nd field! ΔT=0.07 K ------------- 1000 μm ΔT=0.37 K ------------- 125 μm ΔT=1.35 K -------------------- 50 μm ΔT=1.00 K ------------------ 50 μm Red line shows last discernible branch location.**Capillary-mediated branching**bias fields Stefan interface balance advance/retard, Δvn branching! modulation • Analysis: circle, ellipses, parabola, hyperbola, . . . • Applied local equilibrium (GTH) on non-equilibrium analytic shapes • Tangential interface fluxes • Flux divergences • Roots (sign change)**Initial Interface Shapes(Isometric Views)**Ellipse, 2:1 Circle, R=1 a crystal melt crystal melt**GTH Potentials**Ellipse 2:1 Circle**Tangential Fluxes**Ellipse 2:1 Circle**Bias Fields**Ellipse 2:1 Circle**Energetics & Dynamics**• Simulation • Integral eqn. solver • Stefan interface balance • Observed rotation points • Pattern limit cycles**Energy Conservation: Stefan balance**Latent heat Bias Field Bulk energy conduction Fast microscopic processes Slow macroscopic processes Interface modulation eqn: melt crystal**Bias Field Nodes**advance retard retard advance advance retard retard advance**Circle Dendrite**(ε=0.005)**Last discernible branch**Branch initiation (estimated) ΔT=70 mK 1000 microns**Semi-ellipse**(ε=0.005)**Conclusions**Pattern complexities in iridescent butterfly wings and dendritic crystals are interesting and controlled branching provides technological applications. Conventional wisdom attributes pattern branching to noise and stability. NASA-supported microgravity experiments demonstrate that capillary potentials (local equilibria) provide weak interfacial fluxes. Vector flux divergences imply energy release or removal (biases) on interface. Nodes in the bias-field correspond to zeros of the surface Laplacian of the interface potential, a 4th-order function of the interface shape. Positive bias energy retards interface speed, negative bias accelerates it. Local changes in interface curvature couple with the external field and produce branching. Synchronization of bias nodes with interface advance can lead to limit cycles, and dendritic growthif anisotropy is present. Isotropic (fluid-fluid) interfaces evolve by chaotic dynamics, yielding complex ‘seaweed’ patterns.**Acknowledgments**Thank you for listening! Special thanks go to Professors John Lowengrub, Mathematics Dept., U. California, Irvine, CA, and Shuwang Li, Dept. of Applied Mathematics, IIT, Chicago, IL for their efforts in providing noise-free sharp interface dynamics proving the existence of local bias fields.